Surface Functionalization of Silica and Zirconia Sol-Gel Materials with
Nina Danchova, Stoyan Gutzov*
Sofia University “St. Kliment Ohridski”, Faculty of Chemistry and Pharmacy, Department of Physical Chemistry,
J. Bourchier Blvd. 1, 1164 Sofia, Bulgaria * - email@example.com
Keywords: silica, europium complexes, luminescence, sol-gel, zirconia
The present contribution is focused on the relation preparation – structure – optical properties of hybrid silica and zirconia powders containing Eu(III) complexes: [Eu(ntac)3][pphendcn] and
[Eu(phen)2](NO3)3. Methods for functionalization of silica and zirconia microparticles, based on
adsorption of 1,10-phenantroline and [Eu(ntac)3][pphendcn], and doping with [Eu(phen)2](NO3)3
nanoparticles are proposed to obtain of red emitting hybrid composites with quantum efficiency 20 – 50 %. The optical properties of rare earth ions incorporated in silica and zirconia composites are used to explore the site symmetry (D2, C2v or lower) of the Eu3+ optical centers in the hybrid
composites. Quantum yields of the investigated sol-gel micropowders and quantification of their optical spectra are presented.
Sol-gel materials functionalized with rare earth ions and their complexes display important optical properties like luminescence, coloration and energy transfer and give opportunity for wide technical applications as light sources, materials for UV – and IR energy conversion and optical sensors [1,2,3]. As a red emission source Eu(III) complexes with organic ligands are the most often used materials due to their pure, red emission with maxima at about 590 nm, 615 nm, 650 nm and 700 nm [1-4]. From materials science point of view sol-gel species functionalized with rare earth ions are hybrid materials as they contain an organic ligand or complex in an inorganic matrix. Sol-gel chemistry is the most utilized method for preparation of the inorganic matrixes because of the possibilities of low temperature preparation conditions, molecular level of doping and processing of powders, aerogels or monoliths .
Doping of ceramic matrixes /silica, zirconia, alumina, tin oxides/ with europium (III) complexes is a complicated process. If a classic case of sol-gel doping is used, the hybrid optical active specie, here an europium complex, is introduced in the silica containing sol [6,8,9]. Often, europium complexes used in the preparation of hybrid gel composites decomposes during sol-gel process, leading to a low red emission intensity of the obtained sol-sol-gel hybrid composites together with an additional blue or violet emission .
This paper deals with preparation strategies of silica and zirconia gels doped with europium complexes, avoiding decomposition of the europium complexes during sol-gel doping. We are presenting three methods for preparation of strong emitting zirconia or silica samples including: a) physical adsorption of [Eu(ntac)3][pphendcn] on silica surface b) chemical adsorption of
1,10-phenathroline on the surface of europium doped silica and c) incorporation of Eu(phen)2(NO3)3·nH2O colloidal nanocrystals in zirconia sol-gel material.
Here, the following notation is used: [Eu(ntac)3][pphendcn] containing
4,4,4-trifluoro-1-(naphthalene-2-yl) butan-1,3-dione (Hntac) and pyrazino[2,3-f][1,10-phenathroline-2,3-dicarbonitrile (pphendcn) is a new europium complex, detailed described in [5, 6, 7, 8, 9, 10, 11]. The quantum efficiency of the solid complex is 10-15% [6-10]. Eu(phen)2(NO3)3·nH2O, europium
(III) diphenathroline nitrate, is a well-known solid luminescent complex, detailed described in the paper of Mirochnik et al . The quantum efficiency of the solid complex is 35-40%. The room temperature solubility of Eu(phen)2(NO3)3·nH2O in ethanol is 4.5·10-5 mol/l, the solubility of
The europium complexes [Eu(phen)2](NO3)3 and [Eu(ntac)3][pphendcn] were synthesized
according procedures discussed in . A SpectraPro 300i spectrophotometer was used for measurement of diffuse reflectance, excitation / luminescence spectra and quantum yield of powdered samples. As standard, the Lumogen T Rot GG from BASF with maximum wavelength of excitation at 350 nm and maximum wavelength of emission at 615 nm was chosen. The Quantum Yield (QY) of the investigated samples was determined using the comparison method. Emission spectra were integrated between 430 and 750 nm and excitation spectra between 235 and 430 nm. The luminescence and reflectance measurements were used to estimate the QY (defined as the ratio of the number of photons emitted to the number of photons absorbed) of investigated samples. In this study, the presented luminescence spectra are mathematically threated as overlapping Gaussion curves to obtain relative intensities, peak number, peak maxima and half widths of each luminescence peak. The Eu – content in all samples prepared was checked using a ICP Ultima2 Horiba-Jobin Yvon unit.
Emission and excitation spectra with a higher resolution at about 1 nm were measured on a Varian Cary Eclipse fluorescence spectrophotometer with a self-made vertical sample holder, detailed described in . To obtain the peak number in the region of each Stark multiplet second derivative luminescence spectra deconvolution has been applied. All peak maxima detected in this paper were in agreement with the electronic transition of Eu3+ ion .
To prepare silica and zirconia microparticles with an intense red emission, three physico - chemical functionalization techniques, described below, were used.
A) Surface functionalization of silica micro particles with [Eu(ntac)3][pphendcn] (physical functionalization)
The preparation of hybrid silica micro composites includes the following basic steps:
1. Preparation of SiO2 matrix, using a classical base catalyzed sol-gel process, Danchova &
Gutzov (2013) .
2. Homogenization of the solid matrix in mortar to obtain silica micro particles in size 100-300 μm.
3. Impregnation of silica micro particles with solution of 0.0107M [Eu(ntac)3][pphendcn]
4 B) Preparation of functionalized micro particles starting from SiO2:Eu (chemical
The preparation includes the following basic steps:
1. Synthesis of doped SiO2:Eu3+ sol-gel bulk materials with molar ratio nEu/nSi=0.05 using
the procedure of Danchova & Gutzov (2013) .
2. Homogenization of silica gel in mortar to obtain SiO2:Eu3+ silica micro particles
3. Impregnation of doped SiO2 micro particles with ethanol solution of 1.1M
1,10-phenanthroline (48 h at room temperature with molar ratio nEu/nphen = 9.4·10-3,
nSi/nphen= 0.18 .
4. Washing the micropowders with absolute ethanol to remove the excess amount of ligand.
C) Incorporation of Eu(phen2)(NO3)3·xH2O nanoparticles in to a zirconia sol, followed by gelation. [5 6 7 8]
The preparation of hybrid silica micro composites includes the following basic steps: 1. Preparation of a stable zirconia sol, using acetic acid as a complex forming agent to
prevent fast hydrolysis and gelation.
2. Preparation of Eu(phen2)(NO3)3·xH2O following the procedure, described in our
recent paper 
3. Addition of the fresh sol, containing Eu(phen2)(NO3)3·xH2O nanoparticles to the
Zr(IV) sol and gelation of the system.
3. Experimental results and discussion
In Fig. 1. luminescence and excitation spectra of solid SiO2:[Eu(ntac)3][pphendcn],
prepared using the method of physical adsorption are presented. The relative intensity of the Eu3+ 5D
0→7F2 transition is about 83-85%. In the terms Eu3+ site symmetry / spectra correlation, the
most probable site symmetry in SiO2:[Eu(ntac)3][pphendcn] is D2 because of the lack of intensity
in the region of the 5D
0→7F0 emission transition of the Eu3+ ion . It is interesting that the site
5 site symmetry in solution or in solid [Eu(ntac)3][pphendcn] is C2 or lower. In the spectra of solid
[Eu(ntac)3][pphendcn] a relatively intense emission line in the region of the5D0→7F0 emission
transition of the Eu3+ ion together with three lines in the region of the 5D
0→7F1 and five lines in
0→7F2 transition which reveal the site-symmetry of the activator ion . That means that
during physical adsorption the complex structure is changed most probably because of the occurrence of surface interactions.
Figure 1. Luminescence (2) and excitation (1) spectra of SiO2:[Eu(ntac)3][pphendcn]
micropowders, prepared using the method of physical adsorption of a [Eu(ntac)3][pphendcn]. The
0→7Fj transitions are shown as 0-0, 0-1, 0-2, 2-3 and 0-4.
In Fig. 2. a typical luminescence / excitation spectrum of SiO2:[Eu(phen)2](NO3)3 powders
produced from SiO2:0.05Eu3+ using adsorption of 1,10-phenanthroline (chemical
functionalization) is presented. The relative intensity of the Eu3+5D
0→7F2 transition is high, about
80-82% from the overall Eu3+ luminescence intensity between 570 nm and 750 nm. It follows from
6 is C2v . Formation of [Eu(phen)2](NO3)3 as a result of the functionalization of silica and
zirconia with 1,10–phenanthroline has been confirmed by X-Ray diffraction by comparing diffraction patterns of pure solid complexes and functionalized silica samples.
Figure 2. Typical luminescence (2) and excitation (1) spectra of SiO2:[Eu(phen)2](NO3)3
powders produced from SiO2:0.05Eu3+ functionalized using chemical adsorption of
1,10-phenanthroline. The Eu3+ 5D
0→7Fj transitions are shown as 0-0, 0-1, 0-2, 2-3 and 0-4.
Figure 3. presents luminescence / excitation spectra of ZrO2: Eu(phen)2](NO3)3 prepared
using the method of doping with Eu(phen)2](NO3)3·nH2O colloidal nanocrystals. The relative
intensity of the color giving transition 5D
0→7F2 is about 80%. The most probable activator
7 Figure 3. Luminescence (right) and excitation (left) spectra of ZrO2: Eu(phen)2](NO3)3
prepared using the method of doping with Eu(phen)2](NO3)3·nH2O colloidal nanocrystals. The
8 Figure 4. Second derivative luminescence spectra deconvolution of ZrO2:
Eu(phen)2](NO3)3, confirming the most probable site symmetry of the activator ion. The peaks in
the region of each Stark multiplets are shown. The Eu3+ 5D
0→7Fj transitions are shown as 0,
0-1, 0-2, 2-3 and 0-4.
The luminescence emission of the prepared samples SiO2:[Eu(phen)2](NO3)3
SiO2:[Eu(ntac)3][pphendcn] and ZrO2: Eu(phen)2](NO3)3 is very stable for long period of times
(more than 1 year). The excitation spectra in figures 1-3 follow the absorption spectra of the organic ligands and unambiguously prove the occurrence of a very effective energy transfer in the prepared hybrid composites.
9 results in table 1. allow the potential application of the described hybrid powders as potential UV – sensors and label materials for chemical and biological applications.
Table 2 presents a quantification of the Eu3+ luminescence spectra, using three empirical
parameters, described in our recent papers . The parameter P1gives the intensity ratio between the integrated intensities of the electric – dipole transition I5D0→7F2 at 615 nm and the intensity of
the magnetic dipole transition I5D0→7F1 at about 590 nm and the intensity. It is well known, that P1
is high in the case of non-centrosymmetric environment of Eu3+ [4-6].
The relative intensity of another Eu3+ transition, 5D
0→7F0 at 580 nm is also important in
the Eu3+ spectra – structure correlation. It has been pointed out in the study of Binnemanns et al
, that 5D
0→7F0 can be distinguished in the luminescence spectra only if europium ion has a
site symmetry C2v or lower. To describe more accurately the site symmetry in this study, the
parameter P2 is expressed as follows: (2)
1 7 0 5 0 7 0 5 2 F D F D I I P (2)
Here, I5D0→7F1 and I5D0→7F0 are the integrated intensities of the magnetic dipole transition 5D0→7F1
at 590 nm and of the electric dipole 5D
0→7F0 transition at about 580 nm. In table 2. the relative
intensity of the 5D
0→7F2 transition also is given. It is well known, that europium doped optical
materials for laser applications have a high relative intensity of the 5D
0→7F2 transition in the order
Sample / Chemistry
Excitation [nm] QY [%] Eu [%]
Site symmetry of Eu3+
SiO2:[Eu(ntac)3][pphendcn] 400 17.4 0.1 D2
SiO2: [Eu(phen)2](NO3)3 352 39.6 5.4 C2V
ZrO2: [Eu(phen)2](NO3)3 350 48 2.55 C2V
Table 1. Excitation wavelengths, quantum yields (QY) and europium content of the investigated powdered samples at 615 nm emission wavelength. The most probable site symmetry of Eu3+ also
Table 2 .
Sample / Chemistry P1
SiO2:[Eu(ntac)3][pphendcn] 8 0.03 82
SiO2: [Eu(phen)2](NO3)3 8 0.29 83
ZrO2: [Eu(phen)2](NO3)3 8 0.24 85
Table 2. Quantification of Eu3+ luminescence spectra using three parameters: the intensity
parameters P1 and P2 and the relative intensity of the color giving transition Irel5D0-7F2 at 615 nm.
In the case of SiO2:[Eu(ntac)3][pphendcn] having D2 symmetry P2 is very low while in the case of
C2V symmetry (SiO2: [Eu(phen)2](NO3)3 and ZrO2: [Eu(phen)2](NO3)3) the value of P2 is
In this paper the functionalization of sol-gel silica and zirconia microparticles with [Eu(ntac)3][pphendcn] and [Eu(phen)2](NO3)3 complexes using different physico-chemical
11 discussed. All the functionalized samples show a pure, stable in time red luminescence at UV – excitation with quantum yield between 10% and 40% due to energy transfer from organic ligands to the Eu3+ ion. The site symmetry of the Eu3+ ion in the prepared hybrid composites is
non-centrosymmetrical, D2 or C2v.
The authors thank M. Bredol and S. Stoyanov for luminescence spectra measurements.
1Reisfeld, R., Optical materials, 16, 2001, 1-7
2Tanner, P., Yan, B., Zhang , H., Journal of Materials Science 35, 2000, 4325
3Chen, D., Yan, Y., Westengerg, E., Niebauer, D., Sakaitani , and. Chaudhuri, S., Journal of Sol-Gel Science and Technology 19 , 2000, 77 - 82
4Blasse, G., Grabmaier, B., Luminescent materials, Springer, 1994
5 Petkova, N., Dlugocz, S., Gutzov, S., J. Non Cryst. Solids, 357, 2011, 1547
6 Petkova, N., Gutzov, S., Lesev, N., Kaloyanova, S., Stoyanov, S., Deligeorgiev, T. Optical
Materials, 33, 2011, 1715
7 Danchova, N., Gutzov, S., J Sol-Gel Sci Technol, 66, 2013, 248
8 Danchova, N., Gutzov, S., Matras-Postolek, K., Bredol, M., Lesev, N., Kaloyanova, S.,
Deligeorgiev, T., Journal of Inclusion Phenomena and Macrocyclic Chemistry, 78, 2014, 381
9 Danchova, N., Gutzov, S., Z. Naturforschung, 69b, 2014, 224
10 Georgieva, I., Danchova, N., Gutzov, S., Trendafilova, N., J Mol Model, 18, 2011, 2409 11 Mirochnik, A.G., Buktevskii, B.V., Zhikhareva, P.A., Karasev, W.E. Russian Chemical Bulletin
Edition, 51, 2002, 1715
12 Gutzov S., Stoyanova P., Balashev K., Danchova N., Stoyanov S., Bulgarian Chemical
Communications, 3, 2015, in press.